Development of Acoustic Barriers Mainly
Composed of Co-Combustion Bottom Ash
Celia Arenas1, Luis F. Vilches1, Hctor Cifuentes2, Carlos Leiva1,
Jos Vale1, Constantino Fernndez-Pereira1
1 University of Seville, School of Industrial Engineering, Department of Chemical and Environmental Engineering, Camino de los Descubrimientos s/n E-41092, Seville, Spain. Tel:+34-954482274; fax: +34-9554461775. E-mail address: firstname.lastname@example.org 2 University of Seville, School of Industrial Engineering, Continuum Mechanics and Structural Analysis Department, Camino de los Descubrimientos s/n E-41092, Seville, Spain. KEYWORDS: bottom ash, sound absorption coefficient, leachability, radioactivity ABSTRACT
The environmental problem of acoustic pollution is gaining increasing importance for our society. Furthermore, the accumulation of bottom ash and the need for waste management are becoming more and more pressing. This study presents sound absorption and environmental results (leachability EN 12457-4, NEN 7345, and radioactivity tests) for a new product consisting mainly of coal and petcoke co-combustion bottom ash (80 wt %) mixed with Portland cement type II. The combination of three different bottom ash particle size fractions to manufacture a product of 16 cm-thickness which can be used as a panel or noise barrier has been investigated. The acoustic results are similar or even better than those found in porous concrete used for the same application, the mechanical properties are acceptable and the final material presents no environmental risk according to this study.
World of Coal Ash (WOCA) Conference - May 9-12, 2011, in Denver, CO, USA http://www.flyash.info/
Noise is becoming an increasingly significant concern because of its negative impact on human health. Urban traffic noise is one of the most pervasive types of noise pollution. On densely traveled roads the equivalent sound pressure levels for 24h can reach up to 75-80 dB . Changes in the Regulations have led to the creation of programs under the European Directive on the Assessment and Management of Environmental Noise  which are likely to lead to growth in the use of noise barriers as a way of reducing traffic noise. Conventional barriers are generally designed to reflect a large proportion of traffic noise, which creates a problem when a minimization of sound reflection towards noise sensitive areas adjacent to the highway is required. In addition, in the case of residential and other developed areas on both sides of trafficked roadways, pairs of parallel traffic noise barriers are usually set up. However, the multiple reflections occurring between the barriers may end up causing significant degradation of the single barrier screening performance . Therefore, there is a need for traffic noise barriers which absorb noise. These concerns have to lead to major developments in the field of sound absorbing materials . One of the most common materials used for highway noise barrier applications is a combination of lightweight concrete with a hard backing consisting of standard concrete . Lightweight concrete is proportioned by gap grading the coarse aggregates and either eliminating or minimizing the sand volume in the matrix to develop a network of interconnected pores within the material. As a result, the pores inside the material absorb sound energy through internal friction . Many experimental studies have been conducted in the past to develop efficient sound absorbing porous concrete using recycled aggregates as an alternative to normal aggregates . This is due to the fact that as industrial wastes continue to accumulate, they are becoming a major problem for the environment as well as for public health. Moreover, the decrease of natural resources is also becoming a problem. In Spain, over 12% of primary energy consumption came from coal in 2006 , thus large amounts of by-products from coal power plants have been generated. Among them, the uses of fly ash in cement and concrete as a natural pozzolan have been reported in many published articles . However, relatively few detailed studies have been conducted using bottom ash as a replacement material in the production of cement and concrete .
The objective of this study is to design a product composed mainly of bottom ash, reusing all grain particle sizes, so that it can be applied in the field of road noise barriers. The best combination of bottom ash particle grain sizes has been studied in order to achieve the greatest acoustic insulating behavior of the product. An environmental study, including leachability and radioactivity tests, has been carried out to analyze its viability as an outdoor construction element. 2. EXPERIMENTAL WORK
In this study, bottom ash (BA) from the co-combustion of coal and pet-coke (70/30) in a Spanish power plant has been studied. In addition, ordinary Portland cement type II (CPII) (CEM II/B-L 32,5 N according to EN 197-1 ), fine aggregate (Fine) and coarse aggregate (Coarse), in the form of natural river sand and crushed granite were used. The chemical composition of the different materials, according to ASTM D3682-01 , is shown in Table 1, and Figure 1 shows the solids grain size distribution of course materials.
Parameter BA (%) CP II (%) Fine (%) Coarse (%)
SiO2 52.32 13.83 96.21 85.73 Al2O3 25.14 3.53 0.76 4.96 Fe2O3 9.23 2.26 0.22 2.92 MnO 0.07 0.06
Figure 1. Solids grain size distribution (%)
As shown in Table 1, the sum of the percentages of SiO2, Al2O3 and Fe2O3 reaches 87.7 % in the bottom ash, indicating that it can be classified as an F-type ash as prescribed by ASTM C 618 . The calcium content of the bottom ash is very low. The fine and coarse aggregates are fundamentally composed of SiO2; all other analyzed components remaining insignificant. As can be seen in Figure 1, BA presents a higher proportion of fine particles than coarse aggregate, which are mainly composed of larger particles. 2.2 Preparation of test specimens
Our goal was to create a product composed mainly of coal bottom ash, elaborated with all grain particle sizes, and good sound absorption characteristics. For this reason, 16 cm-thick specimens were manufactured, from 80% BA- 20% CPII mortar and combining three different particle sizes. In order to compare the properties of these materials, specimens made from porous (PC) and standard (SC) concrete were also manufactured. Tables 2, 3 and 4 show the compositions of the mortars and their different combinations.
% BA % CPII Particle size (mm) Pattern
BA-C 80 20 > 5
BA-M 80 20 5 > > 1.25
BA-F 80 20 1.25 >
Table 2. Mix proportion (wt% of BA mortars
% Coarse aggregate
aggregate % CPII Pattern
PC 80 - 20
SC 30 50 20
Table 3. Composition (wt%) of porous and standard concrete
The solid components shown in the tables above were placed in a concrete mixer and were mixed until a homogeneous mixture was achieved. Then, water was added to the mixture and it was mixed again until a homogeneous paste was obtained. When the mixing was completed, the paste was placed in moulds and was compacted twice using a vibration table when half-full and full. The pastes were then taken out of the moulds after 24 hours and left to cure at ambient temperature for 27 days (average temperature: 20C; average relative humidity: 95%).
2.3 Test Methods
2.3.1 Acoustic properties
When a sound wave strikes a material, a portion of the sound energy is reflected back, another portion is absorbed by the material while the rest is transmitted. The absorption coefficient, , is the ratio of the absorbed energy to the total incident energy and the reflection coefficient, r, is the ratio of the reflected energy to the total incident energy. To determine the acoustic properties of the products prepared, the sound absorption and reflection coefficients were determined by the impedance tube method  in samples 16 cm thick. The circumferential edge of the test sample was carefully sealed with vaseline, as recommended by the ISO 10534-2, to ensure a good fit between the sample and the tube. A preliminary study was carried out in the impedance tube to analyze the influence of the fit, as in previous studies . Each value represents the average value obtained after testing three samples. The Noise Reduction Coefficient (NRC) was then obtained by calculating the arithmetic mean of the absorption coefficients at 250 Hz, 500 Hz, 1000 Hz and 2000 Hz, in order to make some comparisons. 2.3.2 Physical and mechanical properties
Open void ratio has been measured because this property is related to the acoustic behavior of the products. The method of vacuum water saturation has been followed in the determination of open void ratio (VR %). The samples were oven-dried at 1055C. Subsequently, they were weighed (W1) and left under water in a vacuum vessel until saturation was reached. After 24 hours they were removed and weighed again (W2). The open void ratio was calculated by VR (%) = VW/VS100, where VW is the volume in the sample occupied by water and VS is the total volume of the sample. The volume of water can be found as VW = (W2-W1)/w, where w is the density of water. Density and compressive strength have been measured in order to carry out an exhaustive characterization of the best final product. 10 cm-side cubic test specimens were manufactured. The density () of the mortar was measured by
weight and volume (dimensions) measurements. The compressive strength (Rc) of the test samples was performed based on ASTM C39/C39M-05e2 , using a compressive test machine (Supezcar, MEM-102/50t). Each result was obtained by testing three specimens. 2.4 Environmental study
In order to facilitate its use as a construction material, the product developed in the present study must guarantee a low toxicity level, which is often assessed through a leachability study. The study involved subjecting the different materials to the EN 12457-4 leaching test , at a liquid to solid ratio of 10 L/kg, as well as subjecting the product to one of the most commonly used leaching tests for monolith samples in the waste management field in Europe, the NEN 7345 diffusion test or tank leaching test . Leachate metal analysis was carried out using Atomic Absorption Spectrophotometry and Inductively Coupled Plasma techniques. The radioactivity of the test samples was measured using a well-type HPGe detector from Canberra with a relative efficiency of 30% and crystal volume of 160 cm3. The samples obtained were collected into a cylindrical holder and sealed with paraffin film. Each sample was measured for at least 25 days after the sample was prepared to establish secular equilibrium between 226Ra and 232Th and their respective radioactive progeny. The 226Ra and 232Th contents were measured through the photopeaks of their daughters: 214Bi (1.760 MeV) and 208Tl (2.614 MeV), respectively, while the 40K content was measured directly via its 1.460 MeV peak. 3. RESULTS AND DISCUSSION
3.1 Acoustic behavior
First, the influence of the BA particle size on the acoustic behavior of the products was investigated. Figure 2 shows the sound absorption and reflection coefficient variation of the products made from different BA particle sizes. As can be seen in Figure 2, the sound absorption coefficient increases when the BA particle size is larger. This fact is explained by the void ratio results for SOL. BA-C (VR=37%), SOL. BA-M (VR=28%) and SOL. BA-F (VR=11%). Smaller particle sizes leave less void space between particles and this produces a lower VR in the product. The sound absorption of a porous material is related to the
energy loss by friction produced in the walls of its holes. Consequently, SOL. BA-C presents the highest values of the sound absorption coefficient for all the frequency ranges. The variation of the reflection coefficient is inversely proportional to the sound absorption coefficient. Therefore, lower reflection coefficients are obtained for larger particle size products. In this case, SOL. BA-F presents the best values of the reflection coefficient compared with the other BA products. In general, a product which presents bad sound absorption behavior will probably be a good reflective material.
Figure 2. Sound absorption and reflection coefficients for
BA products of different particle sizes
In the field of noise barriers, the sound absorption of an acoustic product is considered more important than the sound reflection. However, our goal was to develop a product elaborated with the entire range of BA particle sizes (using the BA as it is produced), although not all of them have the same influence on the acoustic behavior of the product. Therefore, the next stage of this research consisted in manufacturing a composite product using two or three layers prepared using different BA particle size fractions to be used as a sound absorbing barrier, as indicated in Table 4. The aim was to
analyze the influence of having BA-F in the last layer of SOL. BA-C or SOL. BA-M specimens, to conform SOL. BA-CF or SOL. BA-MF products as shown in the diagrams included in Table 4.
Product name Combination diagram
Table 4. Combination diagrams of different product solutions
The improvement of the sound absorption coefficient in the medium and high frequency ranges for SOL. BA-CF and SOL. BA-MF products are presented in Figure 3. As can be seen, for low frequency (
literature  for low frequencies and 10-16 cm product thickness, the speed of the sound wave inside the porous layer is very low. As a result, the energy loss by friction is minimal whether they have a reflective layer or not. On the other hand, for medium and high frequencies, when the sound wave hits the reflective wall it changes its direction so that absorption is increased not only because the friction losses become higher, but also because the reflected and direct waves are coupled. This behavior could explain why some peaks are displaced, and have increased or decreased .
Figure 3. Comparison of sound absorption coefficient in single-layer (BA-C and BA-M) and
double-layer products (BA-CF and BA-MF)
Taking into account the results obtained after the second stage, to manufacture an acoustic product elaborated with all the BA particle sizes, the finest material of BA should be used in the last layer of the product (opposite the sound front). In this way, it will probably improve the sound absorption at medium and high frequencies, but will not affect the behavior at low frequencies. Finally, to completely define the acoustic product achieving our goal of using all the BA fractions, it is necessary to identify the composition of...